- Home
- Documents
- A Stochastic Multiscale Model for Microstructure Model ... Stochastic Multiscale Model for Microstructure Model ... A Stochastic Multiscale Model for Microstructure Model Reduction ... RESPONSIBLE PERSON a.

Published on

12-Mar-2018View

216Download

4

Embed Size (px)

Transcript

A Stochastic Multiscale Model for Microstructure ModelReduction

Bin Wena, Nicholas Zabarasa

a Materials Process Design and Control Laboratory, Sibley School of Mechanical and AerospaceEngineering, Cornell University, Ithaca, NY 14853-3801, USA

Abstract

The mechanical properties of a deformed workpiece are sensitive to the initial mi-

crostructure. Often, the initial microstructure is random in nature and location specific.

To model the variability of properties of the workpiece induced by variability in the

initial microstructure, one needs to develop a reduced order stochastic input model for

the initial microstructure. The location-dependence of microstructures dramatically in-

creases the dimensionality of the stochastic input and causes the curse of dimension-

ality in a stochastic deformation simulation. To quantify and capture the propagation

of uncertainty in multiscale deformation processes, a novel data-driven bi-orthogonal

Karhunen-Loeve (KL) decomposition strategy is introduced. The multiscale random

field representing random microstructures over the workpiece is decomposed simul-

taneously into a few modes in the macroscale and mesoscale. The macro modes are

further expanded through a second-level KL expansion to separate the random and

spatial coordinates. The few resulting random variables are mapped to the uniform

distribution via a polynomial chaos (PC) expansion. As a result, the stochastic input

complexity is remarkably simplified. Sampling from the reduced random space, new

microstructure realizations are reconstructed. By collecting the properties of work-

pieces with randomly sampled microstructures, the property statistics are computed. A

high-dimensional multiscale disk forging example of FCC nickel is presented to show

the merit of this methodology, and the effect of random initial crystallographic texture

Corresponding author: N. Zabaras, Fax: 607-255-1222, Email: zabaras@cornell.edu, URL:http://mpdc.mae.cornell.edu/

Preprint submitted to Comput. Mater. Sci. December 19, 2011

Report Documentation Page Form ApprovedOMB No. 0704-0188Public reporting burden for the collection of information is estimated to average 1 hour per response, including the time for reviewing instructions, searching existing data sources, gathering andmaintaining the data needed, and completing and reviewing the collection of information. Send comments regarding this burden estimate or any other aspect of this collection of information,including suggestions for reducing this burden, to Washington Headquarters Services, Directorate for Information Operations and Reports, 1215 Jefferson Davis Highway, Suite 1204, ArlingtonVA 22202-4302. Respondents should be aware that notwithstanding any other provision of law, no person shall be subject to a penalty for failing to comply with a collection of information if itdoes not display a currently valid OMB control number.

1. REPORT DATE 19 DEC 2011 2. REPORT TYPE

3. DATES COVERED 00-00-2011 to 00-00-2011

4. TITLE AND SUBTITLE A Stochastic Multiscale Model for Microstructure Model Reduction

5a. CONTRACT NUMBER

5b. GRANT NUMBER

5c. PROGRAM ELEMENT NUMBER

6. AUTHOR(S) 5d. PROJECT NUMBER

5e. TASK NUMBER

5f. WORK UNIT NUMBER

7. PERFORMING ORGANIZATION NAME(S) AND ADDRESS(ES) Cornell University,Sibley School of Mechanical and AerospaceEngineering,Materials Process Design and Control Laboratory,Ithaca,NY,14853

8. PERFORMING ORGANIZATIONREPORT NUMBER

9. SPONSORING/MONITORING AGENCY NAME(S) AND ADDRESS(ES) 10. SPONSOR/MONITORS ACRONYM(S)

11. SPONSOR/MONITORS REPORT NUMBER(S)

12. DISTRIBUTION/AVAILABILITY STATEMENT Approved for public release; distribution unlimited

13. SUPPLEMENTARY NOTES

14. ABSTRACT The mechanical properties of a deformed workpiece are sensitive to the initial microstructure. Often, theinitial microstructure is random in nature and location specific. To model the variability of properties ofthe workpiece induced by variability in the initial microstructure, one needs to develop a reduced orderstochastic input model for the initial microstructure. The location-dependence of microstructuresdramatically increases the dimensionality of the stochastic input and causes the ?curse of dimensionality?in a stochastic deformation simulation. To quantify and capture the propagation of uncertainty inmultiscale deformation processes, a novel data-driven bi-orthogonal Karhunen-Loeve (KL) decompositionstrategy is introduced. The multiscale random field representing random microstructures over theworkpiece is decomposed simultaneously into a few modes in the macroscale and mesoscale. The macromodes are further expanded through a second-level KL expansion to separate the random and spatialcoordinates. The few resulting random variables are mapped to the uniform distribution via a polynomialchaos (PC) expansion. As a result, the stochastic input complexity is remarkably simplified. Sampling fromthe reduced random space, new microstructure realizations are reconstructed. By collecting the propertiesof workpieces with randomly sampled microstructures, the property statistics are computed. Ahigh-dimensional multiscale disk forging example of FCC nickel is presented to show the merit of thismethodology, and the effect of random initial crystallographic texture on the macroscopic properties.

15. SUBJECT TERMS Stochastic multiscale simulation, multiscale model reduction, location-dependent microstructure,bi-orthogonal decomposition, Karhunen-Loeve expansion, polynomial chaos expansion, property variability.

16. SECURITY CLASSIFICATION OF: 17. LIMITATION OF ABSTRACT Same as

Report (SAR)

18. NUMBEROF PAGES

42

19a. NAME OFRESPONSIBLE PERSON

a. REPORT unclassified

b. ABSTRACT unclassified

c. THIS PAGE unclassified

Standard Form 298 (Rev. 8-98) Prescribed by ANSI Std Z39-18

on the macroscopic properties.

Key words: Stochastic multiscale simulation, multiscale model reduction,

location-dependent microstructure, bi-orthogonal decomposition, Karhunen-Loeve

expansion, polynomial chaos expansion, property variability.

1. Introduction

For polycrystalline materials (e.g. metals, alloys, etc.), macroscale properties are

sensitive to the underlying microstructure. In this work, we are interested in model-

ing the variability of properties of the workpiece in a deformation process induced by

variability in the initial microstructure. To accurately evaluate the properties of a given

microstructure at a given material point, homogenization strategy over a statistical vol-

ume element (SVE) [1, 2, 3] has been widely applied. In the context of polycrystalline

materials, an SVE is a microstructure containing finite number of grains (see Fig. 1)

with features (grain and texture distribution) that satisfy certain statistical constraints.

Given a number of correlated realizations of the microstructure, a stochastic data-driven

model of the microstructure is produced that when coupled with uncertainty quantifi-

cation methods (e.g. Monte Carlo or sparse grid methods) can be used to compute

the distribution of properties at the material point. However, in order to investigate the

variability of macroscopic properties in a workpiece due to microstructure randomness,

we need to exploit the stochastic space of initial microstructures in the workpiece and

not simply at a material point.

Microstructure uncertainty at a material point has been extensively studied using a

variety of methods. In [4, 5] the principle of maximum entropy (MaxEnt) was used to

describe the microstructure topology of binary and polycrystalline materials. A set of

correlation functions or grain size moments were given as the prescribed constraints.

Realizations of microstructures were then sampled from such MaxEnt distribution and

interrogated using appropriate physical model, e.g. a crystal plasticity finite element

method (CPFEM) [6] for polycrystals. The Monte Carlo (MC) method was adopted

to find the error-bars of effective stress-strain response of FCC aluminum. In [7], the

orientation distribution function (ODF) was adopted to describe the polycrystalline mi-

2

crostructure. A number of ODF samples were given as the input data. Karhunen-Loeve

expansion (KLE) [8, 9] was utilized to reduce the input complexity and facilitate the

high-dimensional stochastic simulation. An adaptive version of sparse grid collocation

strategy [10, 11] was used to find the stress-strain curve with error bars and the convex

hull of elastic modulus of FCC aluminum after deformation. Mechanical response vari-

ability and thermal properties due to both orientation and grain size uncertainties were

studied in [12, 13]. A nonlinear model reduction technique based on manifold learn-

ing [14] has been introduced to find the surrogate space of the grain size feature while

grain orientations were reduced by KLE. Critical stress distribution after deformation

was constructed for FCC nickel [12] and effective thermal conductivity distribution

was explored for crystals with ortho-symmetry [13]. Recently, variability of fatigue

resistance, measured by strain-based fatigue indicator parameters (FIPs) [15] of two-

phase nickel-based superalloys was studied with the assistance of principal component

analysis (PCA) [16]. Distributions of FIPs, as well as their convex hulls showing the

extreme values, of microstructures sharing identical statistical features with given sam-

ples under cyclic loading were extracted. Convergence with increasing dimensionality

of the reduced-order representation was also shown.

To quantify the effect of microstructures on macro-properties and probe the un-

certainty propagation through different length scales, a multiscale simulator needs to

be adopted. Each point of the workpiece is associated with a microstructure in the

mesoscale, the deformation of which is controlled by the local deformation gradient

estimated in the macroscale. Mechanical properties/response of the point are evalu-

ated via proper (e.g. crystal plasticity) constitutive model applied on the deformed

microstructure. Since microstructures are random, properties of the workpiece are also

random. In general, microstructures are location-specific (meaning that microstruc-

tures associated with different spatial points may have different distributions) [17]. As

a result, the stochastic input to the probabilistic multiscale forging simulation will be

extremely high dimensional, which prevents one from quantifying the uncertainties of

interested properties. This problem is usually referred to as the curse of dimensional-

ity. Conventional model reduction schemes that only locally decompose input com-

plexity within a single scale and cannot see the correlation between macroscale points

3

are not sufficient for reducing the multiscale stochastic input. To this end, we intro-

duced a bi-orthogonal KLE strategy [18, 19], which decomposes the multiscale random

field into a few modes in both the macro- and meso-scales [20]. Mean and standard

deviation of elastic moduli, i.e. Youngs modulus, shear modulus, and bulk modulus,

over the product were investigated given texture (orientation distribution) uncertainty

of FCC copper microstructures. However, this earlier work limited its stochastic in-

put to two prescribed random variables. In this work, we will build the bi-orthogonal

KLE on the basis of a given set of microstructure data. Different types of macroscale

inner products are discussed. A second-level KLE is conducted to further reduce the

dimensionality of the stochastic space after bi-orthogonal decomposition. The optimal

dimensionality of the final reduced-order space will be determined based on the energy

proportion captured by the principal components in the two-step decomposition. A

non-intrusive strategy is used to project the reduced random variables to the space of

random variables with known probability distributions. Low order statistics of equiv-

alent stress, strain, and strength fields of disks after forging are studied by repeatedly

calling the deterministic solver using microstructures sampled in the reduced space.

We use Monte Carlo (MC) sampling to construct the stochastic solution.

The rest of the paper is organized as follows. In Section 2, the representation of

microstructure and the multiscale forging simulator are introduced. Theory and formu-

lation of the bi-orthogonal KL decomposition, followed by a second-level KLE to fur-

ther decompose the resulting spatial-random coupled modes, will be enunciated in Sec-

tion 3. The reduced microstructure representations are mapped to a multi-dimensional

uniform distribution via polynomial chaos expansion (PCE) so that sampling of mi-

crostructures becomes efficient. The detail of this procedure is presented in Section 4.

Problem definition and generation of initial samples are described in Section 5. Sec-

tion 6 shows an example of stochastic multiscale modeling of nickel disk forging. Prop-

erties/response variability of the product will be investigated. Finally, conclusions and

discussion are given in Section 7.

4

2. Multiscale Modeling of a Forging Process

To study the variability of mechanical properties induced by microstructure un-

certainty in forging disks, a multiscale framework which couples finite element (FE)

large deformation simulator with crystal plasticity constitutive model is introduced as

the deterministic solver. Each point in the macroscale is linked to a mesoscale poly-

crystalline microstructure described by its grain size and orientation features. The me-

chanical properties and response of the material under deformation are evaluated in the

microstructure domain and returned to the workpiece.

2.1. Multiscale Forging Solver

An updated Lagrangian implicit FE model for the analysis of large deformation

forging processes is employed for the multiscale simulation. This model, seamlessly

integrating kinematic, contact, and constitutive modules, is suitable for forging problem

of any material subjected to various die shapes. A crystal plasticity model is used in this

work. Each point (effectively, Gauss integration point) of the macroscale workpiece is

represented by a polycrystalline microstructure whose deformation is controlled by the

local deformation gradient F, while the mechanical properties/response (e.g. effective

stress, strain, strength, etc.) at that point are evaluated in the mesoscale and returned

to the workpiece after homogenization [21]. The multiscale framework is summarized

below.

Macroscale: Let X be a material particle in the initial configuration B0 and x =

x(X, tn+1) be its location at time tn+1. The total deformation gradient defined as

F(X, tn+1) = 0x(X, tn+1) =x(X, tn+1)

X, (1)

can be expressed as the product of Fn at the previous time step t = tn and the relative

deformation gradient Fr:

F = FrFn. (2)

The equilibrium equation at t = tn+1 is expressed in the reference configuration Bnas

n Prh + fr = 0, (3)

5

where n denotes the divergence in Bn. fr ca...